HAL Id: hal-02922544
Submitted on 22 Jan 2021
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.
The role of pre-nucleation clusters in the crystallization
of gold nanoparticles
Raj-Kumar Ramamoorthy, Ezgi Yildirim, Enguerrand Barba, Pierre Roblin,
Jorge A. Vargas, Lise-Marie Lacroix, Isaac Rodríguez-Ruiz, Philippe Decorse,
Valeri Petkov, Sébastien Teychené, et al.
To cite this version:
Raj-Kumar Ramamoorthy, Ezgi Yildirim, Enguerrand Barba, Pierre Roblin, Jorge A. Vargas, et al..
The role of pre-nucleation clusters in the crystallization of gold nanoparticles. Nanoscale, Royal Society
of Chemistry, 2020, 12 (30), pp.16173-16188. �10.1039/d0nr03486j�. �hal-02922544v2�
OATAO is an open access repository that collects the work of Toulouse
researchers and makes it freely available over the web where possible
Any correspondence concerning this service should be sent
to the repository administrator:
This is an author’s version published in:
To cite this version:
Ramamoorthy, Raj Kumar
and Yildirim, Ezgi and Barba, Enguerrand and
and Vargas, Jorge A. and Lacroix, Lise-Marie and
and Decorse, Philippe and Petkov, Valeri and Teychené,
and Viau, Guillaume The role of pre-nucleation clusters in the
crystallization of gold nanoparticles. (2020) Nanoscale, 12 (30). 16173-16188.
The rote of pre-nucleation clusters in the
crystallization of gold nanoparticlest
Raj Kumar Ramamoorthy,
.c Ezgi Yildirim,
a Enguerrand Barba.a
Pierre Roblin,b Jorge A. Vargas,
.e Lise Marie Lacroix,
Isaac Rodriguez Ruiz,
lippe Decorse,' Valeri Petkov,
and Guillaume Viau
The syntheses of metal nanoparticles by reduction in apolar solvents in the presence of long chain surfac tants have proven to be extremely effective in the control of the particle size and shape. Nevertheless, the elucidation of the nucleation/growth mechanism is not straightforward because of the multiple rotes played by surfactants. The nucleation stage, in particular, is very difficult to describe precisely and requires in situ and time-resolved techniques. Here, relying on in situ smalt angle X-ray scattering (SAXS), X-ray absorption spectroscopy (XAS) and high-energy X-ray diffraction (HE-XRD), we propose that ultra-smalt gold particles prepared by reduction of gold chloride in a solution of oleylamine (OY) in hexane with triisopropylsilane do not follow a classical nucleation process but result from pre-nucleation clusters (PNCs). These PNCs contain Au(m) and Au(1) precursors; they are almost stable in size du ring the induction stage, as shown by SAXS, prior to undergoing a very fast shrinkage during the nucleation stage. The gold speciation as a function of time deduced from the XAS spectra has been analyzed through multi-step reaction pathways comprising both highly reactive species, involved in the nucleation and growth stages, and poorly reactive species acting as a reservoir for the reactive species. The duration of the induction period is related to the reactivity of the gold precursors, which is tuned by the coordination of OY to the gold complexes, white the nucleation stage was found to depend on the size and reactivity of the PNCs. The rote of the PNCs in determining the final particle size and structure is also discussed in relation to previous studies. The multiple rotes of OY, as the solubilizing agent of the gold sait, the ligand of the gold complexes determining both the size of the PNCs and the reactivity of the gold precursors, and finally the capping agent of the final gold particles as oleylammonium chloride, have been clearly established. This work opens new perspectives to synthesize metal NPs via metal-organic PNCs and to define new syn thesis routes for nanoparticles that may present structure and morphologies different from those obtained by the classical nucleation routes.
•université de Tou lause, IAboratoire de Physique et Chimie des Nano Objets UMR 5215 INSA, CNRS, UPS, 135 avenue de Ranguei� F 31077 Toulouse cedex 4, France. Email: rajrk37@gmailcom, guillaum.e.viau@insa toulouse.fr
Intense research has been carried out over the past 20 years on
the growth of metallic nanoparticles (NPs) by liquid phase pro
cesses for a precise control of the particle size, 1 shape,2
surface chemistry3 opening applications in biology,4
In this field, huge progress has been
made, for example, on the use of heterogeneou s nucleation by
seed-mediated growth methods.7•8
Until recent times, the for
mation of metal NPs in solution has been described by the
classical nucleation/growth theoiy but several studies stressed
on the possibility of non-classical nucleation pathways depend
ing on the chemical and physico-chemical conditions of the
Detailed knowledge of the nucleation mechanisms
is of paramount importance for the control of the particle mor
phology.10 However, due to its stochastic nature, observing
"IAborawire de Génie Chimique, Université de Toulouse, CNRS, /NP, UPS Toulouse, France.Email: sebastien.teychene@wulouse inp.fr
'Fédération de Recherche FERMaT, Université de Toulouse, CNRS, TNP, INSA, UPS, Toulouse, France
4Department of Physics, Central Michigan University, Mt. Pleasan� MI 48858, USA 'Unidad Académica de Fisica, Universidad Autonoma de Zaazteazs, Calz. Solidaridad esq. Paseo de la Bufa sin, Zaaztecas, Mexico
1université de Paris, ITODYS UMR 7086, 15 rue Jean Antoine de Baif, 75013 Paris, France
tElectronic supplementary infonnation (ESI) available. See DOi: 10.1039/ d0nr03486j
third step of crystallization of the metal particles.28 Formation of dense liquid droplets in which the nucleation and coalescence of the first nuclei occur was observed in the classical citrate synthesis of gold nanoparticles using atomic force microscopy (AFM), dynamic light scattering (DLS) and SAXS.29,30 Such intermediate structures are not specific to aqueous solutions. In organic solvent media, unreduced mesoscopic structures were also identified by DLS in the case of reduction of gold chloride in a solution of oleylamine in octadecene.31
Among the diﬀerent methods, the synthesis of metal nano-particles in apolar solvents, using long alkyl chain surfactants to control the colloidal stability of the final suspensions, is nowadays a very popular method, for both noble32and non-noble metals.33The major property sought in alkyl chain sur-factants is their role in controlling the growth step, leading to a fine control of the particle size and shape.34 However, capping agents such as long chain carboxylic acids35or long chain amines36are also ligands of the metal precursors. The stability of metal complexes, their structure, their self-organiz-ation and their solubility are all factors that can play a deter-mining role in the reaction, the latter therefore depending on the surfactant concentration and on their association constant with the metallic ions. Disentangling the multiple roles of the surfactants at the diﬀerent stages of the reaction is an impor-tant task to improve control over particle morphology and to have a better understanding of their nucleation/growth mechanism.14,37
Gold chloride reduction in oleylamine (OY) solution in hexane, with triisopropylsilane as the reducing agent, is a very simple method to synthesize at room temperature Au NPs with original properties. This is a unique method to synthesize monodisperse ultrathin gold nanowires with very high yield38 that has been used by several groups with applications in diﬀerent fields, such as transparent electronics.39–41By varying
the OY concentration, it is also possible to prepare ultrasmall nanospheres by the same method and, interestingly, regard-less of their shapes both kinds of particles synthesized at room temperature exhibit an atomic structure diﬀerent from the fcc structure of bulk Au.42
In this paper, we present a detailed description of the role of OY in the nucleation/growth mechanism of Au NPs relying on in situ XAS, SAXS and high-energy X-ray diﬀraction (HE-XRD) studies performed during syntheses carried out with diﬀerent OY concentrations. Only a few experimental studies were devoted to the nucleation and growth mecha-nism of NPs prepared by these methods, and exclusively to nanowires characterized using in situ techniques, SAXS,43,44 DLS,45or a combination of XAS and SAXS.46Here, the specia-tion of Au in the diﬀerent oxidaspecia-tion states was deduced from the time-resolved XAS spectra. The speciation with diﬀerent OY concentrations was analyzed through multi-step reaction pathways comprising highly reactive species involved in the nucleation and growth stages and poorly reactive species acting as a reservoir for the reactive species. The reactivity of the diﬀerent species and the “size” of the reservoirs have experimentally the homogeneous nucleation stage can be
extremely challenging and requires in situ and real time tech-niques, such as a combination of in situ X-ray absorption (XAS) and small angle X-ray scattering (SAXS)11 or in situ electron microscopy.12
In the classical nucleation theory (CNT), nucleation is the crossing of the activation energy barrier, resulting from the contribution of the volume and surface to the free energy of the nuclei. In the case of the synthesis of metal particles in solution by the reduction of a metal precursor, the CNT assumes the formation of zero-valent metal atoms and the clustering of these atoms, nucleation being the event when the clusters reach the critical size. This size is obtained when the concentration of the zero-valent atoms exceeds the super-saturation threshold. After the nucleation step, these critical size nuclei further grow. Considering an atom-by-atom growth, the final particle size is given by the nucleation rate. Experimental studies on gold nanoparticles, combining SAXS and UV-visible spectroscopy or XAS, have shown a very good agreement with the CNT.13–15 In addition, thanks to kinetic modeling, these studies have identified the surface reaction as the limiting step of the particle growth. The formation of silver nanoparticles studied by in situ electron microscopy was found to follow the classical nucleation with the existence of a nucleation threshold.12
In the case of metal nanoparticles, an alternative model to the CNT has been proposed, in which the nucleation does not require a supersaturation threshold of zero-valent metal atoms, but occurs via the successive formation of dimers, trimers … and then clusters. The nanoparticle growth is then described by an autocatalytic process at the surface of the metal clusters.16 In that case, the separation between the nucleation and the growth stages is attained if the growth rate is much higher than the nucleation rate.17 A slightly diﬀerent pathway consists in the formation of partially reduced clusters followed by their reduction into zerovalent metal clusters.18,19 In the case of Au NPs synthesized by reduction of gold chloride with citric acid in the presence of PVP, such a pathway via complex clusters has been supported experimentally by XAS showing a progressive contraction of the Au–Au distance during the nucleation stage, followed by a further increase during the growth stage.20
Several recent reviews described non-classical nucleation processes involved in the crystallization of bulk solids and nanoparticles.21–25 These processes occur via more complex free-energy landscapes than the single nucleation barrier of the classical theory, involving stable pre-nucleation clusters (PNCs), as in the case of CaCO3,26 or metastable intermediate
states with an amorphous structure, as in the case of YVO4:
Eu.27 Few examples of non-classical nucleation have been described in the case of metal nanoparticles. An in situ elec-tron microscopy study revealed the formation of gold par-ticles from a homogeneous solution, through three clearly identified stages: an initial spinodal decomposition of the solution into metal-rich and metal-poor phases, a conden-sation of amorphous clusters in the metal-rich phases and a
TIPS can be formally considered as a hydride. The stoichio-metry of the chemical reduction of HAuCl4by TIPS in the
pres-ence of OY can be written as:
HAuCl4þ 3 2R3SiHþ 5 2C18H35NH2 ! Auð0Þ þ3 2R3SiClþ 5 2C18H35NH3 þCl ð1Þ
Thus, TIPS was always introduced in very large excess with respect to the stoichiometry. The experimental conditions with [OY] = 50 mM correspond to the stoichiometry while with [OY] = 100 mM and 400 mM OY was introduced in excess.
In situ experiments. For the in situ SAXS and XAS experi-ments (see below), 3 mL of a solution containing HAuCl4·3H2O (40 mM) and OY (100 mM, 200 mM or 800 mM)
dissolved in hexane and 3 mL of a TIPS (2 M) solution in hexane were prepared. The chemical reduction was achieved by injecting an equal volume of HAuCl4/OY solution and TIPS
solution, at a rate of 10 ml min−1, in a T-micromixer (IDEX-HS P-712) using PHD 22/2000 syringe pumps (Harvard apparatus). The mixing time, estimated from the Falk and Commenge cor-relation, is 40 ms.47The reactions were carried out in a glass capillary and in a PMMA cuvette for SAXS and XAS analysis, respectively (see Scheme S1 in the ESI†).
Au(I) intermediate compound. HAuCl4·3H2O (20 mM) was
dissolved in pure OY (5 mL) and left at room temperature for 48 h. A white precipitate that appeared is a lamellar phase as already described in ref. 44. In the present study, this com-pound has been used as a Au(I) reference for XAS analysis. The
in situ X-ray absorption spectrum at the Au LIII-edge of this
compound was correctly fitted with approximately two N at a distance of 2.09 Å (Table 1). More details about the XAS spec-trum and Extended X-ray Absorption Fine Structure (EXAFS) fit are given in the ESI (Fig. S7†). The presence of only two light atoms in the Au coordination sphere and the atomic ratio Au/ Cl = 1 measured by XPS confirmed that Au has the oxidation state +1 in this compound.
Table 1 Coordination number, N, bond length, R, and Debye Waller factor, σ2, of theﬁrst coordination shell around Au ﬁtted to EXAFS spectra of Au(III) precursors, Au(I) intermediate phase, Au(0) nanospheres and nanowires and gold foil. Figures in brackets indicate the uncertainties of the last digit as estimated afterﬁtting FT EXAFS over three diﬀerent q ranges
NAu–Cl RAu–Cl(Å) σ2Au–Cl(Å2) NAu–N RAu–N(Å) σ2Au–N(Å2)
[OY] 50 mM 4.1(2) 2.23(1) 0.005(1) [OY] 100 mM 1.5(1) 2.28(1) 0.005(1) 2.5(1) 2.02(1) 0.005(1) [OY] 400 mM 4.1(6) 2.06(1) 0.006(2) Au(I) intermediate Au(I) OY 2.1(1) 2.09(1) 0.004(1) NAu–Cl RAu–Cl(Å) σ2
Au–Cl(Å2) NAu–Au RAu–Au(Å) σ2 Au–Au(Å2)
NSs [OY] 50 mM 0.7(1) 2.41(1) 0.004(1) 8.5(5) 2.84(1) 0.014(1)
NWs [OY] 400 mM 0.8(1) 2.37(1) 0.009(1) 9.0(4) 2.86(1) 0.011(1)
Au foil reference 12 2.88(1) 0.008(1)
been interpreted as dependent on the OY coordination at the Au complexes. The time-resolved SAXS study has revealed the presence of pre-nucleation clusters (PNCs) which are involved in the nucleation stage and the size of which depends on the OY concentration. A short Au–Au distance observed in the HE-XRD pattern of the PNCs has been interpreted as an auro-philic bond. The role of PNCs in determining the final par-ticle size and structure is discussed.
Experimental details2.1 Synthesis
Gold nanoparticles. Chemicals were used as received for all syntheses: hydrogen tetrachloroaurate trihydrate (HAuCl4·3H2O, 99.99%, Alfa Aesar), triisopropylsilane (TIPS,
98%, Sigma-Aldrich), oleylamine (OY, 80–90%, Acros) and hexane (mixed isomer, 98+%, Alfa Aesar). Syntheses of Au nanospheres and nanowires were performed by reduction of HAuCl4·3H2O by TIPS in a solution of OY in hexane
follow-ing the procedures described in ref. 42. For all syntheses, the final nominal concentration of Au and TIPS in hexane was kept constant at 20 mM and 1 M, respectively. OY con-centration was varied from 50 mM to 400 mM. HAuCl4·3H2O
was dissolved in 2 mL of solution of OY in hexane. For the lower concentration of OY, the precursor suspension was sonicated for 5 min to help the dissolution. The Au/OY solu-tion in hexane is pale yellow and orange color for the lowest and the highest concentrations of OY, respectively. Then, 512 µL of TIPS was added into the Au/OY solutions. By mixing the TIPS, the solution containing 50 mM OY turns from pale yellow to dark brown-red within few seconds while the solutions containing 100 mM and 400 mM OY take around 10 min and a few hours, respectively, to reach the same color. The particles prepared with [OY] = 50 and 100 mM were analyzed after 3 h of reaction, and the par-ticles prepared with [OY] = 400 mM were analyzed after 24 h of reaction.
resolved SAXS signals were recorded at two distances of 6.07 m and 0.5 m using an Eiger X 4 M (Dectris). Each reaction was performed twice with the SAXS detector at the two diﬀerent distances. For further analysis, the SAXS signals recorded at the two distances were merged in the region q = 0.15–0.2 Å−1.
The nice overlap of the SAXS signals recorded from the two detector positions, all along the reaction time, indicated the reproducibility of the reactions. SAXS patterns, before and after the nanoparticle nucleation, were analyzed with a Beaucage model,48 using a homemade python script. The detailed description of the fitting model and the procedure are presented in the ESI.†
In situ energy dispersive XAS experiments were carried out at the ODE beamline (SOLEIL, France). The XAS was recorded at the Au LIII-edge in transmission mode. Due to
the low concentration of Au, a PMMA cuvette of 10 mm was employed for XAS studies. Time-resolved XAS signals were recorded every 0.36 s for the syntheses with [OY] = 50 and 100 mM and 3.8 s for the syntheses with [OY] = 400 mM. Athena49and Larch50software modules were used for extrac-tion and best-fitting of the EXAFS spectra, respectively. The software PrestoPronto51was used for the linear combination analysis (LCA) of the XAS spectra. EXAFS spectra were Fourier transformed (FT), over three diﬀerent q ranges, 2 Å−1– 8.5 Å−1, 2.5 Å−1–8.5 Å−1 and 2 Å−1–9.0 Å−1, using the Hanning window and fitted in “R” space to extract the first and second shell EXAFS parameters, along with the uncer-tainty values, around the Au absorber. The amplitude and phase shift functions of Au–Cl and Au–N bonds and of Au– Au were calculated from the structure of the aminochloroau-rate(III), AuCl3NH3 (crystallographic open database file no.
1532148),52 and from bulk fcc Au, respectively, using FEFF8.4.53The time-resolved XAS spectrum of each synthesis was analyzed by LCA with three spectra: precursor solution, intermediate compound and final gold particles. This method provided an assessment of the gold speciation as a function of time. More details are given in the ESI.†
In situ HE-XRD experiments were carried out at the 11-ID-B beamline (Advanced Photon Source, Argonne). Samples were contained in thin-walled glass capillaries. The particles were analyzed in suspension in the mother liquor. X-rays with an energy of 58.62 keV (λ = 0.2115 Å) were used, and the scattered intensities were collected with a large area (amorphous Si) detector. The patterns covered wave vectors in the range of 1 Å−1to 25 Å−1with a q-space resolution proven acceptable for atomic pair distribution function (PDF) studies. The acqui-sition time was 1 min for each spectrum, ruling out the possi-bility of monitoring the reaction in real time for [OY] = 50 mM. HE-XRD data for an empty capillary and pure solvents were taken separately and used to correct the HE-XRD patterns for the Au suspensions. Several structure models were tested to describe the experimental PDFs. The models were relaxed in terms of energy and then equilibrated at room temperature by classical molecular dynamics (MD). Best MD models for Au NPs and NWs were refined against the experimental data with a reverse Monte Carlo technique.
2.2 Ex situ characterization
Ex situ transmission electron microscopy (TEM) images were captured using a JEOL-JEM 1400 instrument at an operating voltage of 120 kV. The colloidal suspensions were diluted in hexane and one drop was deposited on a TEM grid covered with a thin carbon film. Ex situ X-ray photoelectron spec-troscopy (XPS) spectra were recorded using a K-Alpha+ system
(ThermoFisher Scientific, East-Grinsted, UK) fitted with a micro-focused and monochromatic Al Kα X-ray source (1486.6 eV, spot size of 400 µm). The spectrometer pass energy was set to 150 and 40 eV for the survey and the narrow high resolution regions, respectively. Several drops of the colloidal suspension prepared with the lowest OY concentration were deposited on a silicon substrate. For the nanoparticles prepared with [OY] = 100 and 400 mM, the excess of OY was removed from the sus-pensions. The colloidal suspensions (1 mL) were mixed with absolute ethanol (3 mL) and centrifuged at 4000 rpm for 5 min. The supernatant was discarded and the particles were re-dispersed in pure hexane. Several drops of the purified sus-pensions were deposited on a Si substrate. Ex situ X-ray diﬀrac-tion (XRD) at wide angles was carried out on a Panalytical Empyrean diﬀractometer equipped with a Co Kα X-ray source, a Bragg–Brentano HD primary optics and a linear Pixcel1D detector. The nanoparticles were centrifuged at 4000 rpm for 5 min after addition of an OY solution in absolute ethanol (3 mL) to the mother liquor (1 mL). The supernatant was dis-carded and the particles were redispersed in a small volume of hexane. Several drops of the particle suspensions were de-posited on a zero-background silicon substrate and dried in air. The patterns were recorded with a step size of 0.8° and a time per step of 250 s.
2.3 In situ studies
SAXS, XAS and HE-XRD measurements were performed in a static mode, during and after the completion of a reaction. For the kinetic studies, the glass capillaries and PMMA cuvettes were filled using the mixing procedure described in section 2.1 for the synthesis of gold nanoparticles. In the case of 2.5 mL PMMA cuvettes for XAS experiments, the dead volume was 0.75 mL (Scheme S1 in the ESI†). With a total flow rate of 20 mL min−1, the dead volume was filled after 2.25 s. The first XAS acquisition time after mixing was 4 s. For SAXS experi-ments, the very small dead volume in the capillaries allowed capturing the SAXS signal at the very beginning of the reaction.
In situ SAXS synchrotron experiments were carried out at the SWING beamline (SOLEIL, France) and at the c-SAXS beamline (PSI, Switzerland). SAXS measurements were per-formed in the transmission mode with an X-ray source energy of 12.5 keV and 11.5 keV. A glass capillary with a diameter of 1.5 mm was used for each measurement. In situ SAXS signals were acquired every 2 s for the syntheses with [OY] = 50 and 100 mM, and every 1 min 10 s for the syntheses with [OY] = 400 mM. At PSI, time-resolved SAXS signals were recorded at a distance of 2.17 m using a PILATUS 2 M. At SWING,
time-the final particle size does not vary with time. The nanoparticles observed after 3 h and 24 h exhibit the same mean diameter and same standard deviation of the size distribution (see ESI, Fig. S1†). The nanoparticle morphology is very dependent on the OY concentration. A bimodal distribution of isotropic par-ticles, a major population with a mean diameter of 2.2 and a minor population of 5.9 nm were found for [OY] = 100 mM after 3 h of reaction. The smallest particles self-organized on the TEM grid, while the largest ones are located at the grain bound-aries of the small particle super-lattices (Fig. 1b). For [OY] = 400 mM, the reaction is much slower and the particle growth is completely diﬀerent with the formation of nanowires (NWs) exhibiting a mean diameter of 2.0 nm and length of several micrometers. With the average diameter of the spheres and wires prepared with [OY] = 50 and 400 mM, respectively, being almost the same, the ratio between the volumes of the two types of particles is greater than several thousand. Therefore, oleyl-amine does not only act as a simple capping agent of the final particles but also plays a crucial role in the nucleation rate.
The XRD patterns of the diﬀerent samples exhibited very broad bands in agreement with the very small diameter of the particles (ESI, Fig. S2†). The comparison with the expected positions of the diﬀerent reflections for the fcc structure of Au suggests a structure diﬀerent from the bulk. It is noteworthy that the structure of the synthesized NPs is very diﬀerent from the one of those prepared with ammonium borohydride or amino borane as the reductant that crystallize with the classi-cal fcc structure.13,15Structural models required HEXRD and pair distribution function (PDF) analysis. The experimental PDFs are given in Fig. 2 along with the best fits obtained from the 3D models shown as insets. In order to make a fair com-parison, the PDF of a truncated octahedron nanoparticle with
Fig. 1 Transmission electron microscopy images of nanoparticles and nanowires prepared with diﬀerent concentrations of oleylamine: (a) [OY] = 50 mM, isotropic particles with a mean diameter dm= 2.2 nm (σ/dm=
13%); (b) [OY] = 100 mM, isotropic particles with bimodal size distri bution dm= 2.2 nm (σ/dm= 11%) and 5.9 nm (σ/dm= 21%);(c) [OY] =
400 mM, nanowires with a mean diameter dm= 2.0 nm (σ/dm= 13%).
Particles were deposited on TEM grids after 3 h of reaction (a) and (b), or after 24 h (c).
Fig. 2 In situ atomic pair distribution function of Au nanoparticles pre pared by reduction of HAuCl4·3H2O in OY solution in hexane at diﬀerent
OY concentrations (black circles) and best PDFﬁts (red lines) obtained from the atomic models presented as insets: distorted icosahedron for [OY] = 50 mM, Marks decahedron for [OY] = 100 mM and wire with a tcp structure derived from theα Mn crystal structure. The theoretical PDF of a truncated octahedron with a fcc crystal structure is also given for comparison.
Results and discussion3.1 Au nanoparticle morphology and structure
Fig. 1 shows representative TEM images of the final Au nano-particles, prepared by reduction of HAuCl4·3H2O in solution of
OY in hexane, with a large excess of TIPS, for three diﬀerent OY concentrations. For [OY] = 50 mM, isotropic particles with a mean diameter of 2.2 nm are observed. After 30 min of reaction,
despite the washing. We can thus conclude that the oleyl-ammonium chloride is strongly bound to the gold NP surface, in agreement with adsorption energy calculations.56
3.2 Influence of [OY] on the Au(III) precursor/in situ study of
the Au(III) precursors
The precursor solutions, prepared by dissolution of HAuCl4·3H2O in hexane with diﬀerent OY concentrations, were
studied both by XAS and by SAXS prior to the addition of TIPS. The XAS spectra of the precursor solutions exhibit an intense white line peak “A” at 11 921.2 eV, characteristic of the Au complex in the +3 oxidation state (ESI, Fig. S5a†). An increasing intensity of the feature“C” at 11 934 eV and a slight shift of the white line towards high energy are observed with increasing OY concentration (Fig. S5a,† inset). To evaluate the local changes of the Au coordination sphere in the diﬀerent precursors, the FT of the EXAFS signals was fitted in R-space using the amplitude and phase shift functions of reference files calculated by FEFF8.4 (see Experimental details). The fitted curves of the diﬀerent Au precursors are presented in the ESI (Fig. S5b–d†) and the fit parameters to the first coordination shell are summarized in Table 1. For [OY] = 50 mM, 4 Cl atoms at the distance R = 2.23 Å are found in the first coordination shell of Au. These values are consistent with the formation of [AuCl4]− OY+ ion pairs when
HAuCl4is dissolved in the solution of OY in hexane. As a matter
of comparison, the Au–Cl bond length is between 2.23 and 2.34 Å in the dimer Au2Cl3 in the solid state,57 and takes an
average value of 2.277 and 2.274 Å in NaAuCl4 and NR4AuCl4,
respectively.58,59With increasing [OY], the chlorine atoms of the coordination shell are progressively replaced by nitrogen. A mixed Cl/N coordination shell is found for [OY] = 100 mM and four N atoms as first neighbors are found for [OY] = 400 mM. The bond length RAu–N is found between 2.02 and 2.06 Å
(Table 1). The Au–N bond length is a little bit longer than that in AuCl3NH3,52but similar to the bond length measured by EXAFS
in a solution of HAuCl4in hexane with an excess of OY.46 This
complexation of the Au(III) ions by OY is also revealed by a
change in the color of the solution, from pale yellow with [OY] = 50 mM to dark orange with [OY] = 400 mM.
The SAXS patterns of the diﬀerent precursor solutions are shown in Fig. 3. Whatever the OY concentration, the scattering intensity exhibits a Guinier regime in the intermediate-q region and a Porod regime in the high-q region. Since the organic molecules, OY and TIPS, exhibit almost the same scattering length density (SLD) as hexane (Table S1†) they cannot be responsible for the scattering intensity at small angles. In con-trast, the SLD of the ion pair [AuCl4]−OY+and the one of gold
chloride coordinated with OY are estimated as almost twice the SLD of hexane (Table S1†). Thus, the observed scattering inten-sity is interpreted as the presence of molecular clusters of Au(III)
complexes in solution. These clusters will be further referred to as pre-nucleation clusters (PNCs). Note that in the case of [OY] = 100 mM, the increasing intensity at very small q can reveal the presence of secondary structures resulting from the assembly of PNCs (Fig. 3). Two variations in the SAXS profiles are observed when [OY] is increased. The “knee-feature” is shifted toward a fcc structure is presented in the same figure. It is clear that
none of the Au nanoparticles synthesized here exhibits a fcc structure. The agreement between the experimental and simu-lated PDFs is remarkable allowing us to talk about the atomic ordering with confidence. The nanoparticles obtained with [OY] = 50 and 100 mM are well described by distorted icosa-hedra and Marks decaicosa-hedra, respectively, while the nanowires obtained with [OY] = 400 mM exhibit a distinctive lack of the fcc second neighbor distance about r = 4 Å, also present in ico-sahedral and decahedral structures. This led us to propose a tetrahedrally close packed structure derived from the α-Mn structure incorporating distorted icosahedra and larger size coordination polyhedra, as reported in our previous work.42
According to the first feature of the PDFs, the first-neighbor Au–Au pair distance is found at about 2.86 Å, which is slightly smaller than the Au–Au bonding distance in bulk Au (2.88 Å).
The XAS at the Au LIII-edge of nanospheres and nanowires
are given in Fig. S3 of the ESI† with the fits to the EXAFS spectra. The coordination number (N), the bond distance (R) and the Debye–Waller factor (σ2) deduced from these fits are
given in Table 1. Two distinct atom shells were needed to fit the EXAFS spectra. Around the Au absorber, 0.7 Cl and 8.5 Au atoms, and 0.8 Cl and 9 Au atoms are found for the nano-spheres and the nanowires, respectively (Table 1). Under the same conditions, the NAu–Au coordination number was found
to be equal to 12 in the Au foil, as expected for the bulk metal with a fcc structure. The lower NAu–Au coordination number
determined here in both cases is related to the small particle diameter. For 2.2 nm gold NPs, 50% of the Au atoms are located at the surface and therefore are uncoordinated. For the nanowires, the relative amount of undercoordinated surface atoms was estimated as 43%.42 The Au–Au distances of 2.84 Å
and 2.86 Å found in the nanospheres and nanowires, respect-ively, are in good agreement with the PDF results and previous XAS studies on ultrasmall gold particles.20,54
The XPS survey scans of the particles prepared with [OY] = 50 mM exhibited Au 4f, C 1s, N 1s, and Cl 2p peaks centered at ca. 84, 285, 400, and 198 eV, respectively (ESI, Fig. S4†). The Au 4f7/2 and 4f5/2 high-resolution spectra were fitted with a single
component corresponding to Au(0). The N 1s high-resolution spectrum revealed a main peak centered at 401.3 eV corres-ponding to the binding energy of oleylammonium cation N atoms.55 The molar ratio ammonium/chlorine calculated from the integrated intensity of the two respective peaks was found to be equal to 1 in agreement with the formation of the oleyl-ammonium chloride. A minor peak, centered at 399.2 eV, corresponds to the binding energy of oleylamine N atoms. The relative intensity of OY represented only 7% of the total N 1s intensity showing that for the molar ratio Au/OY = 2.5, the con-version of OY into ammonium is almost complete in agree-ment with the stoichiometry of eqn (1). For the nanospheres and nanowires prepared with an excess of OY, the N 1s high-resolution spectrum exhibited two contributions centered at the same energy of 401.3 and 399.5 eV.43 Under such
con-ditions, only a part of OY was converted to ammonium which was nevertheless clearly identified in the XPS spectrum,
results. To assess the gold speciation as a function of time, time-resolved XAS spectra were fitted by the linear combination analyses (LCA), as described in previous studies.14,31At first, the LCA were performed with only two contributions, the spec-trum of the Au(III) initial precursor at t = 0 s (Fig. S5a†) and the
one of the final Au(0) nanoparticles after 24 h of reaction (Fig. S3a†). Nevertheless, the best fits of the XAS spectra left out a significant residual contribution. Based on previous growth mechanism studies44,60,61 showing that a Au(I) phase
with a layered structure could be an intermediate in the reduction of gold tetrachloride in the presence of oleylamine, the XAS spectrum of such an Au(I) phase (Fig. S7 in the ESI†),
prepared with a large excess of oleylamine (see the Experimental section), was introduced as a third possible con-tribution in the LCA. An example of LCA is given in Fig. 4b showing the goodness of the fit. For each XAS spectrum, the relative weights of the three diﬀerent components were deduced from the LCA and were attributed to the gold concen-tration in the three diﬀerent oxidation states. The relative con-centrations of Au(III), Au(I) and Au(0) are plotted for a short
time range (up to 120 s) and for a longer time range (up to 25 min) in Fig. 4c and d, respectively. Three stages can be defined: the induction period, the nucleation, and the growth stage. Straight after the addition of TIPS, Au(I) is observed in
the medium. The first stage, until 10 s, is referred as the induc-tion period, during which the reducinduc-tion from Au(III) to Au(I) is
noticed. The second stage corresponding to the onset of Au(0) and then to the steep increase of Au(0) concentration, grey shaded area in Fig. 4c, is interpreted as the nucleation stage. During this period, the Au(I) concentration reaches the
maximum value of ca. 35%. After t = 30 s, the increase of [Au(0)] is slowed down which is interpreted as the end of the nucleation and the beginning of the growth stage. 50% of the gold precursor has reacted during the first 30 s and the remain-ing 50% is reduced very progressively durremain-ing the followremain-ing several tens of minutes. In order to describe more precisely the nucleation/growth stages and to assess the reaction rates, an autocatalytic model was defined following Finke’s approach.16
However, a model taking into account only the two-step reduction, Au(III)→ Au(I)→ Au(0), and the auto-catalytic step,
Au(I) + Au(0) → Au(0), was not able to describe both the very
rapid variations of [Au(III)] and [Au(0)] during the nucleation
stage and the very slow ones during the growth stage. The study on the Au(III) complexes with diﬀerent OY concentrations
showed that OY can coordinate the Au ions. In the reaction with the molar ratio [OY]/[Au] = 2.5, one equivalent of OY is used to dissolve HAuCl4 in hexane through the formation of
the ion pair OY+[AuCl4]−. The 1.5 equivalents of OY remaining
in solution can complex the Au ions and modify their reactivity. Competition between reduction and complexation was there-fore introduced leading to a possible co-existence of reactive Au(III) and Au(I) species (schematically Au coordinated mostly
with Cl) and inert species toward the reduction (schematically complexes with OY in the Au coordination sphere). In this model, the nucleation and the auto-catalytic step involve only the “reactive” Au(I) species (Scheme 1). The kinetic model is
Fig. 3 SAXS pattern of the initial precursors obtained by dissolving HAuCl4in a solution of OY in hexane at the OY concentrations of 50 mM
(black line), 100 mM (red line) and 400 mM (blue line).
high-q, from about 0.08 Å−1 for [OY] = 50 mM to 0.12 Å−1 for [OY] = 400 mM, and the slope of the Porod regime is decreasing. The radius of gyration, Rg, and the exponent of the power law in
the Porod regime, p, were determined by fitting a Beaucage equation to the SAXS profiles (see ESI, Fig. S6†). Assuming spherical objects, the average diameter was calculated from the relationship DSAXS ¼ 2p5=3Rg. DSAXS was found to decrease
from 4.4 nm for [OY] = 50 mM, to 3.9 nm for [OY] = 100 mM and to 2.7 nm for [OY] = 400 mM (Table S2 in ESI†). The value for the higher [OY] is similar to the one previously reported by Pschunder et al.46 The exponent p for the Porod law decreases from 3.5 to 2.8 for [OY] = 50 mM and 400 mM, respectively (Table S2†). These values reveal surface fractal objects, with an open shape and a rough surface. This confirms the “molecular nature” of the clusters, presumably coordination polymer chains in folded conformation. The decreasing p value indicates that the clusters transform from surface fractal to mass fractal at high [OY]. In other words, a large excess of OY limits the clus-tering and creates less dense zones inside more open clusters. This eﬀect may be related to the increasing number of OY mole-cules coordinated to the Au atoms that can limit the clustering of the gold complexes.
3.3 In situ study of nucleation and growth of Au nanospheres The nucleation and growth of the nanospheres prepared with [OY] = 50 mM were studied by in situ XAS and SAXS to follow both the Au speciation and the particle morphology as a func-tion of time.
Gold speciation. Time-resolved XAS spectra recorded during the synthesis of gold nanoparticles with [OY] = 50 mM are shown in Fig. 4a. Once the addition of TIPS is performed, the EXAFS oscillations are modified, the intensity of the white line at 11 921.2 eV decreases and the intensity of the peak “B” at 11 948.5 eV increases. After 30 min, the XAS spectrum is similar to that of a Au foil, indicating that most of the Au(III)
Scheme 1 Modelling of the reaction mechanism of the Au nanosphere formation with [OY] = 50 mM. The reduction pathway involves a two step reaction, Au(III) to Au(I) and Au(I) to Au(0). The Au(0) NP nucleation/growth process is modelled by an auto catalytic process with the reaction rate
constants kNand kAC. A competition between reduction and complexation of the Au(III) and Au(I) by OY is described by two additional equilibrium
during the induction stage. The two“non reactive” complexes are not directly involved in the reduction steps but serve as a reservoir for the “reactive complexes”.
Fig. 4 (a) In situ XAS spectra at the Au LIII edge recorded during the synthesis of Au nanoparticles in a solution of OY/hexane with [OY] = 50 mM;
(b)ﬁt of the XAS spectrum at 29 s (open circles) by a linear combination of three components (magenta line), Au(III) precursor (black line), Au(I) inter mediate (red line) andﬁnal Au(0) NPs (blue line). Relative Au(III), Au(I) and Au(0) concentrations deduced from the LCA: (c) plotted between 0 and 120
s and (d) between 1.5 and 25 min. The open dots correspond to the bestﬁt to the Au speciation, the symbols (+) correspond to the reactive Au(III) and Au(I) species, and the symbols (×) correspond to the less reactive Au(III) and Au(I) species (see text). (e) Nucleation and growth rates as a function
isotropic shape for the PNCs. The exponent of the power law at high-q is also almost constant with an average value of 3.3 (Table S4†). Thus during the induction stage, a slight shrink-age of the PNC size and almost no change in their internal
Fig. 5 In situ SAXS patterns recorded during the synthesis of Au nano particles in OY/hexane solution with [OY] = 50 mM: (a) between 4 and 40 s and (b) between 48 s and 30 min; (c) particle mean diameter as a function of time, calculated from the radius of gyration of the Au(III) Au(I)
pre nucleation clusters during the induction stage and from that of Au(0) NPs during the growth stage. The grey shaded area corresponding to the nucleation stage was deduced from the XAS results.
described with more details in the ESI (Table S3† and corres-ponding text). As can be seen in Fig. 4(c and d), this kinetic model describes satisfactorily the variation of [Au(III)], [Au(I)]
and [Au(0)] over the entire reaction. The reactive Au(III) species
are consumed very rapidly during the induction and nucleation stages, while the concentration of the reactive Au(I) species
reaches a maximum value just after the onset of Au(0). During the growth stage, the concentrations of the reactive species are almost zero, both the “non-reactive” Au(III) and Au(I) species act
as reservoirs, and their transformation into reactive species is the limiting step of the reaction. Thanks to the modelling of the kinetics, it is possible to plot the nucleation and growth rates as a function of time (Fig. 4e). The rate constants fitted to the gold speciation show an overlap between nucleation and growth during the steep increase of Au(0) and after 35 s the growth rate is higher than 1.9 times the nucleation rate (Fig. 4f). This time is in very good agreement with the extent of the nucleation stage deduced from the experimental curves. It is noteworthy that, experimentally, the beginning of nucleation has been taken at the onset of Au(0), i.e. when particles exhibit-ing a metallic rather than a molecular character appear in the medium because the reference for the Au(0) species in the LCA analysis was gold nanoparticles. It means that the presence of soluble Au(0) species was neglected in our analysis. This stres-ses the limit of the comparison between the gold speciation and the Finke’s model where the nucleation is described by a single step reaction. It may explain the small discrepancy between the experimental data and the modelling at the begin-ning of the nucleation. The modelling was nevertheless very useful to show the presence of non-reactive species and to identify the end of the nucleation stage when VN becomes
much lower than VAC.
Evolution of size – SAXS. Fig. 5 shows the time evolution of the SAXS patterns recorded during the synthesis of nano-particles with [OY] = 50 mM, for the first 40 s of reaction, i.e. covering the induction and nucleation stages and the begin-ning of the growth stage (Fig. 5a), and between 48 s and 30 min, i.e. during the growth stage (Fig. 5b).
The absolute scattering intensity is almost constant between t = 4 s and 22 s i.e. during the induction stage. The SAXS profile is as follows: a Porod regime in the very low-q range, a Guinier regime in the intermediate-q range with a “knee-feature” and a Porod regime in the high-q range (Fig. 5a). This SAXS profile is interpreted from the presence of primary scattering objects responsible for the intensity in high- and intermediate-q ranges, these first level structures being assembled at a larger scale into secondary structures, responsible for the low-q power law. The structure of the primary objects is similar to the PNCs observed prior to the addition of TIPS (Fig. S9a†). The scattering intensity profiles were analyzed using a Beaucage equation48 for a two level
structure in order to take into account the secondary structures (see more details in the ESI, Fig. S9†). The main fitted para-meters to the SAXS curves are given in Table S4.† The radius of gyration is comprised between 17 and 14.8 Å, giving a dia-meter DSAXS that decreased from 4.4 to 3.8 nm, assuming an
Considering that, at these very small sizes, the addition of a 1 atom shell means an increase of 50% in the number of atoms in the particles, the size increase is consistent with the XAS analysis showing that 50% of Au was involved in the growth stage (Fig. 4). The value of the exponent of the high-q Porod regime was fixed to 3.7, equal to that of the 30 min signal. This value is close to 4, the expected value for metal particles with a smooth surface in suspension in liquid. The slight diﬀerence can be attributed to NP surface disorder and/or adsorption of unreduced species at the metal NP surface since the reduction was not complete at 30 min.
Fig. 5c summarizes the overall process including the XAS and SAXS results:– molecular pre-nucleation clusters with an almost stable size during the induction stage;– fast shrinkage of the PNCs in the time interval corresponding to the nuclea-tion stage according to the XAS results;– slow increase of the metal NP mean size during the growth stage. The shrinkage is interpreted as the transition from molecular clusters with a long internal Au–Au distance to dense metal NPs with a shorter internal Au–Au distance.
3.4 Influence of [OY] on kinetics of nucleation and growth Fig. 6(a and b) depict the speciation of gold species in the diﬀerent oxidation states, Au(III), Au(I) and Au(0), for the
synth-eses with [OY] = 100 mM and 400 mM, calculated from the LCA analysis of the time-resolved XAS spectra following the
Fig. 6 Relative Au(III), Au(I) and Au(0) concentrations deduced from LCA of the in situ time resolved XAS spectra at the Au LIII edge during the Au
nanoparticle synthesis with (a) [OY] = 100 mM and (b) [OY] = 400 mM (right). Onﬁgure (b) the open dots correspond to the best ﬁt of the kinetic model to the XAS data, the symbols (+) and (×) correspond to the reactive and less reactive intermediate Au(I) species, respectively (see text). (c)
Nucleation and growth rates as a function of time, given by the kinetic modeling of the Au nanowire synthesis with [OY] = 400 mM, according to reaction Scheme 2; (d) ratio between the growth and nucleation rates of the Au nanowire synthesis with [OY] = 400 mM.
structure are noticed while the XAS study showed a progressive reduction of Au(III) to Au(I) during the same period. Between
22 s and 34 s, i.e. during the period identified as the nuclea-tion stage in XAS, an abrupt change of the scattering intensity profile is observed, with a very fast shift of the “knee-position” to the high-q region. Thus, for the time range corresponding to the highest [Au(0)] slope in the LCA-XAS data, a shrinkage of the particle size occurs that can be interpreted as the fast transformation of the PNCs into metal nuclei. For the period going from 48 s to 30 min, identified as the growth stage, the knee-position is progressively shifting towards low-q and the SAXS intensity in the intermediate-q range is progressively increasing, which is interpreted as a slight increase of the metal nanoparticle size. The scattering intensity profiles during the growth stage were fitted to a sum of two single level Beaucage equations corresponding to a mixture of remaining PNCs and metal NPs (see the ESI for more details, Fig. S9†). The weight of the PNCs scattering intensity, the radius of gyra-tion and the slope of the Porod law corresponding to the SAXS intensity of the metal nanoparticles are reported in the ESI (Table S4†). When time increases, the weight of the PNCs decreases and the metal particle size increases from 1.9 to 2.4 nm (Fig. 5c). These values are consistent with the mean size measured from the TEM images. The metal NP size increase, observed during the growth stage, corresponds approximately to 1 atomic layer around the metal particles.
14 minutes, the scattering intensity increases and the knee-position shifts toward low-q, showing an increasing number of metal nanoparticles with an increasing size. The size of the PNCs and of the metal particles inferred from the fits of the SAXS patterns are given in Table S6.† A change in the scatter-ing intensity of the Porod regime at very low-q is also notice-able between the beginning of the reaction and 30 min (Fig. S12†). The slope at low-q, revealing some secondary struc-tures of the pre-nucleation clusters, is present during the whole induction stage. It vanishes progressively from 15 min, i.e. at the beginning of the growth stage, and has disappeared
Scheme 2 Modelling of the reaction mechanism of the Au nanowires formation with [OY] = 400 mM. The Au(0) NP nucleation/growth process is modelled by an auto catalytic process with the reaction rate constants kNand kAC. The very large excess of oleylamine in the medium favors the for
mation of a“non reactive” Au(III) complex. This complex is progressively reduced into a“non reactive” Au(I) complex in equilibrium with a reactive
Au(I) complex which isﬁnally involved in the Au(0) formation. Both “non reactive” complexes serve as a reservoir for the “reactive complexes”.
Fig. 7 In situ SAXS patterns recorded during the synthesis of Au nano particles in OY/hexane solution: (a) [OY] = 100 mM, during theﬁrst 20 minutes and (b) [OY] = 400 mM.
same method as in the previous section. The corresponding XAS spectra and examples of LCA are reported in the ESI (Fig. S10†). Increasing [OY] prolongs the induction stage, Au(0) appearing after 10 min and around 180 min for [OY] = 100 mM and 400 mM, respectively. In both cases, the onset of Au(0) started when the Au(I) concentration reached the relative
value of about 0.55 and [Au(I)] reached a maximum value of
0.6. Since the final particles have very diﬀerent volumes, it is noteworthy that the nucleation rate is independent of [Au(I)].
An auto-catalytic model was built to describe the kinetics of the reaction with [OY] = 400 mM. For such OY concentration, the gold precursor characterization (section 3.2) showed that the initial solution contained mainly Au complexes co-ordinated by oleylamine. These complexes were considered as poorly reactive for the reduction by TIPS and in equilibrium with poorly reactive Au(I) species. These Au(I) species are
them-selves in equilibrium with reactive Au(I) species involved in the
nucleation and auto-catalytic steps as in the previous model (Scheme 2). The kinetic model is described in a more detailed way in the ESI (Table S4† and corresponding text). As can be seen in Fig. 6b, this model fits very well to the variations of [Au(III)], [Au(I)] and [Au(0)] over the entire reaction. The
nuclea-tion and growth rates given by this model are plotted as a func-tion of time in Fig. 6c. Interestingly, the modelling describes well that the nucleation stage involves only a very small amount of gold, at the opposite of the nucleation stage of the nanospheres prepared with [OY] = 50 mM. The grey shaded area in Fig. 6b corresponds to the nucleation stage. It begins at the onset of Au(0) and finishes when VAC is much higher than
VN. According to the rate constants given by the fit, the growth
rate becomes higher than twice the nucleation rate at 200 min and increases very quickly afterwards (Fig. 6d). The end of the nucleation stage has been taken arbitrarily at t = 200 min.
The time-resolved SAXS patterns recorded during the syn-thesis with [OY] = 100 mM are given in Fig. 7a for the period 4 s–20 min that covers the induction, nucleation and beginning of the growth stages, and in Fig. S12† for the complete reac-tion. The scattering intensity profile due to the 3.9 nm PNCs remains almost constant during the first 5 minutes (Fig. 7a). Between 5 and 14 min, there is a progressive change in the scattering intensity, with the shift of the “knee-position” to high-q. This phenomenon occurs in the time range corres-ponding to the onset of Au(0) in the gold speciation plot. Thus, a shrinkage of the particle size is observed at the metal particle nucleation, similarly to what has been already observed with [OY] = 50 mM, but much slowed down. After ca.
variation of morphology of the scattering objects in solution with the extent of the reaction all along the induction, nuclea-tion and growth stages. HE-XRD has completed the study pro-viding structural information on the precursors before nuclea-tion and on the final gold particles.
The main result that must be highlighted here is the role of the molecular PNCs in the nucleation of the gold particles. PNCs involved in secondary structures were identified by SAXS for all OY concentrations. The PNCs shrinkage observed by SAXS is concomitant with the nucleation and the beginning of growth of the metal particles Au(0) observed by XAS. Moreover, the secondary structures attributed to van der Waals attraction between the PNCs vanish progressively during the nucleation stage. SAXS requires a contrast in the SLD between the clusters and the solvent, high enough to give a significant intensity. It shows that the core of the clusters contains Au(III) and/or Au(I)
complexes. A short Au–Au distance was detected by HE-XRD during the pre-nucleation/induction stage showing an
associ-Fig. 8 In situ atomic PDFs as a function of time: (a) [OY] = 100 mM; (b) [OY] = 400 mM. The blue arrow highlights the Au Au pair distances present at the beginning of the reaction as a PDF peak centered at 3.38 Å; the black arrow highlights the bonds between Au and light atoms, N or Cl, appearing as a broad PDF peak centered at about 2.15 Å; the red dotted arrow highlights the Au Au pair distances in metal NPs appearing as a well deﬁned PDF peak centered at 2.84 Å and 2.86 Å.
after 30 min (Fig. S12†). This observation highlights that the nucleation stage occurs from PNCs involved in larger hierarch-ical structures. The reduction of the PNCs into metal nano-particles destabilizes the secondary structures.
After ca. 40 minutes, a shift to the low-q region of the “knee-position” is observed along with an increasing scattering intensity (Fig. S12†). This last phenomenon was not observed with [OY] = 50 mM and can be interpreted as a secondary growth stage with an increasing number of bigger particles in agreement with the TEM images of the final particles showing a bimodal distribution with particles of diameter 6 nm.
Fig. 7b depicts the SAXS patterns for the synthesis with [OY] = 400 mM. The scattering intensity remains almost constant for the first 150 min. A progressive increase of the scattering intensity at low-q is then observed, in agreement with the growth of nanowires. After around 450 min, the scattering intensity at low q follows a q−1 power law showing that the
dominant scattering objects in the medium are the nanowires.43,46
High-energy X-ray diﬀraction combined with PDF analysis is a good probe for very small particles and/or poorly crystal-line compounds.62 PDFs calculated from the in situ HE-XRD
pattern recorded during the syntheses of the nanoparticles prepared with [OY] = 100 mM and nanowires prepared with [OY] = 400 mM are shown in Fig. 8. For both kinetics, the PDFs exhibit at the beginning of the reaction a distance at 3.38 Å in good agreement with an Au–Au aurophilic bond observed mainly in Au(I) dimers or chains, but also in some
cases in Au(III) dimers.63 For [OY] = 100 mM, after ca. 10 min
of reaction, a well-defined PDF peak at a radial distance of 2.84 Å corresponding to the Au–Au pair distance in metal nanoparticles is also observed. This last distance is in good agreement with the distance measured by EXAFS. The PDF peak at 3.38 Å disappeared rapidly and after 1 h the PDF was similar to the one after 22 h (Fig. 8a). It shows that, after 1 h, the scattering intensity at wide angles is mainly due to the atomic correlation in the metal particles, in agreement with the SAXS and XAS results. For [OY] = 400 mM, the distance at 3.38 Å was observed during the first 150 minutes of reaction, i.e. covering the whole induction stage. Then, this distance progressively disappeared while at the same time progressively appeared the distance at 2.86 Å corresponding to the metal bond in the nanowires, in agreement with the LCA analysis (Fig. 8b). Unfortunately, the acquisition time of few minutes required for a good HE-XRD pattern prevented the study of the structure of the pre-nucleation clusters for the very fast reac-tion with [OY] = 50 mM.
The reduction of gold chloride by the TIPS in hexane in the presence of diﬀerent concentrations of OY leads to ultrasmall gold particles, spheres or wires, with an unusual atomic struc-ture. The OY concentration plays a decisive role in the nuclea-tion and growth stages. The joint XAS and SAXS studies have permitted combining chemical and morphological infor-mation during the nanoparticle synthesis and correlating the
particles shows that the nucleation is an internal reduction of the pre-nucleation clusters.
The second particularity of this system is related to the reduction by TIPS of Au complexes coordinated or partially co-ordinated by OY. The LCA of the time resolved XANES spectra showed the co-existence of the three oxidation states during the growth stage whatever OY concentration, but the reaction rate constants of the diﬀerent reduction steps, deduced from the kinetic modeling, are at least two orders of magnitude smaller for [OY] = 400 mM than for [OY] = 50 mM. This high-lights the role of OY that not only forms an ammonium to dis-solve [AuCl4]−but also changes the reactivity of the precursors
by binding to the Au ions. Kinetic modelling required the introduction of non-reactive Au(III) and Au(I) species to
cor-rectly describe experimental gold speciation. It is known from the literature that gold(I) complexes with amine and chloride
ligands can adopt two kinds of coordination chemistry forming charged or neutral complexes, [Au(RNH2)2]Cl or
(RNH2)AuCl, respectively.64 Both kinds of compounds form
polymeric chains like [Au(NH3)2]X65 or (OY)AuCl.44 In these
chains, the aurophilic bond is reinforced by hydrogen bonds between NH2and Cl groups. With a large excess of OY, the Au
(III)N4 and Au(I)N2 centers were evidenced by EXAFS showing
the complete substitution of the chloride by OY in the Au ion coordination spheres. With a slight excess of OY, the presence of both coordination complexes is very likely.
Eqn (1) that describes the whole reduction of Au(III) to Au
NPs is supported by the absence of molecular hydrogen evol-ution during the syntheses and by the total conversion of oley-lamine to ammonium when it is added in stoichiometric amount. The gold reduction by TIPS involves hydrides as inter-mediates. Gold hydrides have been proposed as intermediates in gold-catalyzed reactions such as hydrogenation66or hydro-silylation.67 Previous studies showed also the possibility to isolate Au(III) and Au(I) hydrides using lithium borohydride68
or hydrosilane viaσ-bond metathesis.69Thus, the first step of Au(III) and Au(I) reduction by TIPS likely proceeds via aσ-bond
metathesis with formation of a gold hydride and triisopropyl chlorosilane, followed by a reductive elimination of a proton with the help of oleylamine to form the ammonium. The sub-stitution of Cl by OY in the coordination spheres of the gold complexes reduces the possibility ofσ-bond metathesis which could be the reason for the lower reduction rates; the reduction then occurs only through a dynamic ligand exchange in the Au coordination sphere. This hypothesis is supported by the need to introduce in the kinetic models equi-libria between reactive (complexes containing chloride in the coordination sphere) and non-reactive species (complexes with only OY in the coordination sphere).
Thus, by substituting the chloride ions in the coordination sphere of the gold precursors, OY has a double eﬀect. It slows down the reduction rates by the TIPS and notably increases the induction times, and it limits the association of the mole-cular complexes into large pre-nucleation clusters limiting the number of nuclei. A third eﬀect of OY that can also contribute to slowing down the reduction rate is the formation of a ation of Au complexes, attributed to the aurophilic bond. The
surface fractal structure of the PNCs may be attributed to the presence of oleylamine in the outer shell. For the highest OY concentration, the internal structure seems quite diﬀerent which could be due to the large number of OY coordinating the Au atoms, thus limiting their association. The size of the PNCs was determined by SAXS but the question then arises on assessing the number of gold atoms constituting the PNCs depending on their size. Assuming a molecular volume of the gold complex coordinated by Cl and OY of about 0.6–0.65 nm3
(Table S1†) and assuming PNCs with a spherical shape, the ratio between the volume of the PNCs and the molecular volume of the gold complex gives from 50 to 70 units in the PNCs with a diameter of 3.9–4.4 nm, like those observed with [OY] = 50 mM, and only 15 units for the PNCs with a diameter of 2.7 nm, like those observed with [OY] = 400 mM. Gathering SAXS and XAS results, a possible description of the Au NP for-mation with [OY] = 50 mM is: (i) a sudden reduction of the PNCs to Au(0) nuclei containing 50 to 65 atoms, i.e. to a size of about 1–1.2 nm; (ii) a very fast growth with remaining highly reactive Au(I) species to give 1.9 nm NPs; (iii) and after 30 s a
slower growth involving the 50% less-reactive species remaining to give finally the 2.4 nm final Au NPs. The numbers of Au atoms inside the PNCs do not take into account possible inhomogeneity of density inside the clusters, such as a core shell structure with OY chains organized as an outer shell. Hence, the molecular volume in the cluster cores could be lower and the number of Au atoms higher, but this does not change the overall description. The same scheme applies to the nucleation and first growth stage of the nanospheres prepared with [OY] = 100 mM. However, in this case, the OY excess increases the non-reactive species amount, the nucleation step involves less Au and an additional growth stage is observed leading to a bimodal size distribution. It is noteworthy, however, that the primary particles have the same size as in the case with [OY] = 50 mM, despite a much slower nucleation rate. This cannot be explained in the framework of the classical nucleation theory, as was mentioned in other systems.27 For
the nanowire synthesis, Pschunder et al. proposed a nucleation involving pre-nucleation clusters and reported on a size con-traction at the nanowire nucleation.46 Here, we show that the
size of the clusters depends on the OY concentration and we can make the hypothesis that the PNC size and the degree of coordination with OY of the Au centers involved in the nuclei determine the nucleation rate. The biggest PNCs appear very reactive, because they contain enough Au atoms to lead to stable nuclei, whereas the smallest ones are not reactive and, as suggested by Pschunder et al.,46 require an association into
bigger anisotropic structures to lead to the nucleation. In both schemes, the Au(0) nuclei are not generated according to the classical nucleation theory, i.e. by the progressive association of Au(0) free monomers into small Au(0) clusters and then stable Au(0) nuclei, as it was described by Abécassis et al.13 or by
Chen et al.15 for the chemical reduction of gold chloride using
borohydride or borane as reductants. In the present case, the shrinkage of the pre-nucleation clusters into small Au(0) metal
The authors thank M. Impéror-Clerc, Laboratoire de Physique des Solide, CNRS-Université Paris Saclay, and Q. Kong, SOLEIL, for fruit full discussions about SAXS and XAS. RKR acknowledges Fédération FERMaT (Université de Toulouse) for financial support during his post-doctoral stint. The authors thank SOLEIL for providing synchrotron radiation facilities at SWING and at ODE beamlines (Proposal No.: 20171002) as well as J. Perez and Q. Kong for the assistance provided for the use of the beam lines. The authors thank PSI, Switzerland, for providing synchrotron radiation facilities at c-SAXS beamline (Proposal No.: E190700304) as well as Ana Diaz for the assist-ance provided for the use of the beam line. This work used resources of the Advanced Photon Source at the Argonne National Laboratory provided by the DOE Oﬃce of Science under contract no. DE-AC02-06CH11357. Thanks are due to Dr K. Beyer for the help with the HE-XRD experiments. This project has received funding from the European Union’s Horizon 2020 research and innovation program under grant agreement no. 731019 (EUSMI). The work was supported in part by DOE-BES grant DE-SC0006877.
1 J. Park, J. Joo, S. G. Kwon, Y. Jang and T. Hyeon, Angew. Chem., Int. Ed., 2007, 46, 4630–4660.
2 D. Huo, M. J. Kim, Z. Lyu, Y. Shi, B. J. Wiley and Y. Xia, Chem. Rev., 2019, 119(15), 8972–9073.
3 M. R. Axet and K. Philippot, Chem. Rev., 2020, 120, 1085– 1145.
4 P. K. Jain, X. Huang, I. H. El-Sayed and M. A. El-Sayed, Acc. Chem. Res., 2008, 41, 1578–1586.
5 A. Kamyshny and S. Magdassi, Small, 2014, 10, 3515–3535. 6 K. An and G. A. Somorjai, ChemCatChem, 2012, 4, 1512–
7 Y. Xia, K. D. Gilroy, H.-C. Peng and X. Xia, Angew. Chem., Int. Ed., 2017, 56, 60–95.
8 W. Niu, L. Zhang and G. Xu, Nanoscale, 2013, 5, 3172–3181. 9 N. T. K. Thanh, N. Maclean and S. Mahiddine, Chem. Rev.,
2014, 114, 7610–7630.
10 E. V. Shevchenko, D. V. Talapin, H. Schnablegger, A. Kornowski, Ö. Festin, P. Svedlindh, M. Haase and H. Weller, J. Am. Chem. Soc., 2003, 125, 9090–9101.
11 J. Polte, T. T. Ahner, F. Delissen, S. Sokolov, F. Emmerling, A. F. Thunemann and R. Kraehnert, J. Am. Chem. Soc., 2010, 132, 1296–1301.
12 T. J. Woehl, J. E. Evans, I. Arslan, W. D. Ristenpart and N. D. Browning, ACS Nano, 2012, 6, 8599–8610.
13 B. Abécassis, F. Testard, O. Spalla and P. Barboux, Nano Lett., 2007, 7, 1723–1727.
14 B. Abécassis, F. Testard, Q. Kong, F. Baudelet and O. Spalla, Langmuir, 2010, 26, 13847–13854.
15 X. Chen, J. Schröder, S. Hauschild, S. Rosenfeldt, M. Dulle and S. Förster, Langmuir, 2015, 31, 11678–11691.
second shell of OY around the coordination sphere of the Au complexes with large OY concentration, limiting the access of the TIPS to the Au(III) and Au(I) coordination sphere. This
hypothesis is supported by the fact that, in a large excess of OY, the final nanowires are surrounded by a bilayer of oleylam-monium/oleylamine, as it was reported in previous studies.43
This bilayer was also described as responsible for the aniso-tropic growth through the formation of cylindrical micelles around the wires. A fourth eﬀect that has not been considered here is the reducing power of OY assuming that Au(III) and Au
(I) complexes are reduced by OY at higher temperature.31
The nucleation/growth mechanism evidenced for the nano-sphere formation can be summarized as follows: formation of non-reduced PNCs; progressive reduction from Au(III) to Au(I)
inside the clusters without significant PNC size modification; abrupt size shrinkage of the PNCs into metal nuclei contain-ing approximately 50–60 atoms; fast growth involvcontain-ing reactive Au complexes followed by a slow growth involving non-reactive complexes acting as a reservoir. In the case of nanospheres, the PNCs are large enough and/or enough reactive to allow the nucleation directly from PNCs. In the presence of an excess of OY the PNCs are smaller and less reactive, limiting the nuclea-tion and slowing down the growth. This mechanism is consist-ent with a previous study on the nanowire formation that described the association of prenucleation clusters into aniso-tropic objects before the metal NW nucleation. The classical nucleation theory does not apply for these systems since the number of nuclei depends more on the size and reactivity of the PNCs rather than on a concentration threshold of zero-valent gold atoms. The multiple roles of OY have been clarified thanks to this study. The complete substitution of chloride ions by OY in the Au coordination sphere not only limits the clustering but also hinders the action of TIPS preventing the formation of hydrides through metathesis.
The PNCs in this study have still an ill-defined formula [AuxClyOYz]n. In future studies, it will be interesting to improve
the structural characterization of the PNCs at the atomic/mole-cular scale. A better assessment of the number of Au atoms involved in the nucleation stage will be useful to complete the mechanism description because the kinetic modeling includ-ing an autocatalytic process, although very useful for demon-strating the presence of non-reactive species acting as reser-voirs, does not include information on the size of the nuclei. A prospect for this work is to extend the study to other systems exhibiting reactive metal–organic PNCs and try defining new rational routes of ultrasmall nanoparticles and ultrathin nano-wires with non-classical structures.